#------------------------------------------------------------------------------
#$Date: 2021-06-01 12:44:07 +0300 (Tue, 01 Jun 2021) $
#$Revision: 265653 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/30/1563052.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1563052
loop_
_publ_author_name
'Gulay, L.D.'
'Daszkiewicz, M.'
'Shemet, V.Ya.'
_publ_section_title
;
 Crystal structure of ∼ RCu3S3 and ∼ RCuTe2 (R=Gd--Lu) compounds
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              142
_journal_page_last               148
_journal_paper_doi               10.1016/j.jssc.2011.12.004
_journal_volume                  186
_journal_year                    2012
_chemical_formula_moiety         'Cu2 Lu0.67 S2'
_chemical_formula_sum            'Cu2 Lu0.67 S2'
_chemical_formula_weight         308.43
_space_group_IT_number           164
_space_group_name_Hall           '-P 3 2"'
_space_group_name_H-M_alt        'P -3 m 1'
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 3 2"'
_symmetry_space_group_name_H-M   'P -3 m 1'
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            1
_cell_length_a                   3.8694(14)
_cell_length_b                   3.8694(14)
_cell_length_c                   6.3263(19)
_cell_measurement_reflns_used    97
_cell_measurement_temperature    295(2)
_cell_measurement_theta_max      27.75
_cell_measurement_theta_min      3.22
_cell_volume                     82.03(5)
_computing_cell_refinement       'CrysAlis RED'
_computing_data_collection       'CrysAlis CCD (Oxford Diffraction, 2009)'
_computing_data_reduction        'CrysAlis RED'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      295(2)
_diffrn_detector_area_resol_mean '1024x1024 with blocks 2x2, 33.133pixel/mm'
_diffrn_measured_fraction_theta_full 0.990
_diffrn_measured_fraction_theta_max 0.990
_diffrn_measurement_device_type  'KUMA KM-4 with area CCD detector'
_diffrn_measurement_method       ω-scan
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0315
_diffrn_reflns_av_sigmaI/netI    0.0149
_diffrn_reflns_limit_h_max       5
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_k_min       -5
_diffrn_reflns_limit_l_max       8
_diffrn_reflns_limit_l_min       -8
_diffrn_reflns_number            1025
_diffrn_reflns_theta_full        27.75
_diffrn_reflns_theta_max         27.75
_diffrn_reflns_theta_min         3.22
_diffrn_standards_interval_count .
_diffrn_standards_interval_time  .
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    33.856
_exptl_absorpt_correction_T_max  0.315
_exptl_absorpt_correction_T_min  0.094
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   'CrysAlis (Oxford Diffraction, 2009)'
_exptl_crystal_colour            red
_exptl_crystal_density_diffrn    6.244
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       prism
_exptl_crystal_F_000             138
_exptl_crystal_size_max          0.10
_exptl_crystal_size_mid          0.05
_exptl_crystal_size_min          0.04
_refine_diff_density_max         1.343
_refine_diff_density_min         -0.995
_refine_diff_density_rms         0.195
_refine_ls_extinction_coef       0.060(8)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.234
_refine_ls_hydrogen_treatment    .
_refine_ls_matrix_type           full
_refine_ls_number_parameters     10
_refine_ls_number_reflns         98
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.234
_refine_ls_R_factor_all          0.0195
_refine_ls_R_factor_gt           0.0191
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0138P)²+0.5694P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0421
_refine_ls_wR_factor_ref         0.0422
_reflns_number_gt                97
_reflns_number_total             98
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            JSSC-2012-186-142.CIF
_cod_data_source_block           lu
_cod_database_code               1563052
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'y, x, -z'
'x-y, -y, -z'
'-x, -x+y, -z'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'-y, -x, z'
'-x+y, y, z'
'x, x-y, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Lu Lu 0.0000 1.0000 0.0000 0.0101(4) Uani 0.67 12 d SP . .
Cu Cu 0.3333 0.6667 0.6279(2) 0.0220(4) Uani 1 6 d S . .
S S 0.3333 0.6667 0.2432(4) 0.0101(5) Uani 1 6 d S . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
S S 0.1246 0.1234 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Lu Lu -0.4720 5.8584 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
S Lu S 180.00(8) 7_565 1_565
S Lu S 91.00(6) 7_565 7_575
S Lu S 89.00(6) 1_565 7_575
S Lu S 89.00(6) 7_565 .
S Lu S 91.00(6) 1_565 .
S Lu S 180.0 7_575 .
S Lu S 91.00(6) 7_565 7_675
S Lu S 89.00(6) 1_565 7_675
S Lu S 91.00(6) 7_575 7_675
S Lu S 89.00(6) . 7_675
S Lu S 89.00(6) 7_565 1_455
S Lu S 91.00(6) 1_565 1_455
S Lu S 89.00(6) 7_575 1_455
S Lu S 91.00(6) . 1_455
S Lu S 180.0 7_675 1_455
S Lu Cu 134.02(2) 7_565 7_676
S Lu Cu 45.98(2) 1_565 7_676
S Lu Cu 134.02(2) 7_575 7_676
S Lu Cu 45.98(2) . 7_676
S Lu Cu 81.06(5) 7_675 7_676
S Lu Cu 98.94(5) 1_455 7_676
S Lu Cu 45.98(2) 7_565 1_454
S Lu Cu 134.02(2) 1_565 1_454
S Lu Cu 45.98(2) 7_575 1_454
S Lu Cu 134.02(2) . 1_454
S Lu Cu 98.94(5) 7_675 1_454
S Lu Cu 81.06(5) 1_455 1_454
Cu Lu Cu 180.0 7_676 1_454
S Lu Cu 134.02(2) 7_565 7_576
S Lu Cu 45.98(2) 1_565 7_576
S Lu Cu 81.06(5) 7_575 7_576
S Lu Cu 98.94(5) . 7_576
S Lu Cu 134.02(2) 7_675 7_576
S Lu Cu 45.98(2) 1_455 7_576
Cu Lu Cu 73.19(3) 7_676 7_576
Cu Lu Cu 106.81(3) 1_454 7_576
S Lu Cu 45.98(2) 7_565 1_554
S Lu Cu 134.02(2) 1_565 1_554
S Lu Cu 98.94(5) 7_575 1_554
S Lu Cu 81.06(5) . 1_554
S Lu Cu 45.98(2) 7_675 1_554
S Lu Cu 134.02(2) 1_455 1_554
Cu Lu Cu 106.81(3) 7_676 1_554
Cu Lu Cu 73.19(3) 1_454 1_554
Cu Lu Cu 180.0 7_576 1_554
S Lu Cu 98.94(5) 7_565 1_564
S Lu Cu 81.06(5) 1_565 1_564
S Lu Cu 45.98(2) 7_575 1_564
S Lu Cu 134.02(2) . 1_564
S Lu Cu 45.98(2) 7_675 1_564
S Lu Cu 134.02(2) 1_455 1_564
Cu Lu Cu 106.81(3) 7_676 1_564
Cu Lu Cu 73.19(3) 1_454 1_564
Cu Lu Cu 106.81(3) 7_576 1_564
Cu Lu Cu 73.19(3) 1_554 1_564
S Lu Cu 81.06(5) 7_565 7_566
S Lu Cu 98.94(5) 1_565 7_566
S Lu Cu 134.02(2) 7_575 7_566
S Lu Cu 45.98(2) . 7_566
S Lu Cu 134.02(2) 7_675 7_566
S Lu Cu 45.98(2) 1_455 7_566
Cu Lu Cu 73.19(3) 7_676 7_566
Cu Lu Cu 106.81(3) 1_454 7_566
Cu Lu Cu 73.19(3) 7_576 7_566
Cu Lu Cu 106.81(3) 1_554 7_566
Cu Lu Cu 180.0 1_564 7_566
S Cu S 108.88(6) 7_676 7_566
S Cu S 108.88(6) 7_676 7_666
S Cu S 108.88(6) 7_566 7_666
S Cu S 110.06(6) 7_676 .
S Cu S 110.06(6) 7_566 .
S Cu S 110.06(6) 7_666 .
S Cu Cu 125.56(3) 7_676 7_566
S Cu Cu 55.97(6) 7_566 7_566
S Cu Cu 125.56(3) 7_666 7_566
S Cu Cu 54.09(5) . 7_566
S Cu Cu 55.97(6) 7_676 7_676
S Cu Cu 125.56(3) 7_566 7_676
S Cu Cu 125.56(3) 7_666 7_676
S Cu Cu 54.09(5) . 7_676
Cu Cu Cu 89.08(7) 7_566 7_676
S Cu Cu 125.56(3) 7_676 7_666
S Cu Cu 125.56(3) 7_566 7_666
S Cu Cu 55.97(6) 7_666 7_666
S Cu Cu 54.09(5) . 7_666
Cu Cu Cu 89.08(7) 7_566 7_666
Cu Cu Cu 89.08(7) 7_676 7_666
S Cu Lu 55.11(4) 7_676 1_656
S Cu Lu 113.44(7) 7_566 1_656
S Cu Lu 55.11(4) 7_666 1_656
S Cu Lu 136.50(2) . 1_656
Cu Cu Lu 169.41(6) 7_566 1_656
Cu Cu Lu 98.44(3) 7_676 1_656
Cu Cu Lu 98.44(3) 7_666 1_656
S Cu Lu 55.11(4) 7_676 1_556
S Cu Lu 55.11(4) 7_566 1_556
S Cu Lu 113.44(7) 7_666 1_556
S Cu Lu 136.50(2) . 1_556
Cu Cu Lu 98.44(3) 7_566 1_556
Cu Cu Lu 98.44(3) 7_676 1_556
Cu Cu Lu 169.41(6) 7_666 1_556
Lu Cu Lu 73.19(3) 1_656 1_556
S Cu Lu 113.44(7) 7_676 1_546
S Cu Lu 55.11(4) 7_566 1_546
S Cu Lu 55.11(4) 7_666 1_546
S Cu Lu 136.50(2) . 1_546
Cu Cu Lu 98.44(3) 7_566 1_546
Cu Cu Lu 169.41(6) 7_676 1_546
Cu Cu Lu 98.44(3) 7_666 1_546
Lu Cu Lu 73.19(3) 1_656 1_546
Lu Cu Lu 73.19(3) 1_556 1_546
Cu S Cu 108.88(6) 7_676 7_566
Cu S Cu 108.88(6) 7_676 7_666
Cu S Cu 108.88(6) 7_566 7_666
Cu S Cu 69.94(6) 7_676 .
Cu S Cu 69.94(6) 7_566 .
Cu S Cu 69.94(6) 7_666 .
Cu S Lu 165.50(10) 7_676 1_545
Cu S Lu 78.91(3) 7_566 1_545
Cu S Lu 78.91(3) 7_666 1_545
Cu S Lu 124.56(4) . 1_545
Cu S Lu 78.91(3) 7_676 .
Cu S Lu 78.91(3) 7_566 .
Cu S Lu 165.50(10) 7_666 .
Cu S Lu 124.56(4) . .
Lu S Lu 91.00(6) 1_545 .
Cu S Lu 78.91(3) 7_676 1_655
Cu S Lu 165.50(10) 7_566 1_655
Cu S Lu 78.91(3) 7_666 1_655
Cu S Lu 124.56(4) . 1_655
Lu S Lu 91.00(6) 1_545 1_655
Lu S Lu 91.00(6) . 1_655
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Lu S 2.7126(15) 7_565
Lu S 2.7126(15) 1_565
Lu S 2.7126(15) 7_575
Lu S 2.7126(15) .
Lu S 2.7126(15) 7_675
Lu S 2.7126(15) 1_455
Lu Cu 3.2455(13) 7_676
Lu Cu 3.2455(13) 1_454
Lu Cu 3.2455(13) 7_576
Lu Cu 3.2455(13) 1_554
Lu Cu 3.2455(13) 1_564
Lu Cu 3.2455(13) 7_566
Cu S 2.3782(12) 7_676
Cu S 2.3782(12) 7_566
Cu S 2.3782(12) 7_666
Cu S 2.433(3) .
Cu Cu 2.7583(18) 7_566
Cu Cu 2.7583(18) 7_676
Cu Cu 2.7583(18) 7_666
Cu Lu 3.2455(13) 1_656
Cu Lu 3.2455(13) 1_556
Cu Lu 3.2455(13) 1_546
S Cu 2.3782(12) 7_676
S Cu 2.3782(12) 7_566
S Cu 2.3782(12) 7_666
S Lu 2.7126(15) 1_545
S Lu 2.7126(15) 1_655
